microstructure and mechanical properties of gypsum ... . 11, no. 4, 2008 microstructure and...
Post on 20-Apr-2018
Embed Size (px)
Materials Research, Vol. 11, No. 4, 391-397, 2008 2008
Microstructure and Mechanical Properties of Gypsum Composites Reinforced with Recycled Cellulose Pulp
Magaly Arajo Carvalhoa*, Carlito Calil Jniora, Holmer Savastano Juniorb,
Rejane Tubinoc, Michele Tereza Carvalhod
aEscola de Engenharia de So Carlos, EESC/USP So Carlos - SP, Brazil bFaculdade de Zootecnia e Engenharia de Alimentos, FZEA/USP, Pirassununga - SP, Brazil
cEscola de Engenharia Civil, EEC/UFG Goinia - GO, Brazil dFurnas Centrais Eltrica Goinia - GO, Brazil
Received: May 20, 2007; Revised: October 17, 2008
The use of waste fibers for the reinforcement of brittle matrices is considered opportune for the sustainable management of urban solid residues. This paper examines the microstructure and mechanical properties of a composite material made of gypsum reinforced with cellulose fibers from discarded Kraft cement bag. Two different kinds of gypsum were used, natural gypsum (NG) and recycled gypsum (RG), both with an addition of 10% by mass of limestone. For the production of samples, slurry vacuum de-watering technique followed by pressing was evaluated revealing to be an efficient and innovative solution for the composites under evaluation. The composite was analyzed based on flexural strength tests, scanning electron microscopy (SEM) imaging, secondary electron (SE) detection, and pseudo-adiabatic calorimetry. The morphology of the fractured surfaces of flexural test samples revealed large gypsum crystals double the original size surrounding the fibers, but with the same overall aspect ratio. Natural fibers absorb large amounts of water, causing the water/gypsum ratio of the paste to increase. The predominance of fiber pullout, damaged or removed secondary layers and incrusted crystals are indicative of the good bonding of the fiber to the gypsum matrix and of the high mechanical resistance of composites. This material is a technically better substitute for the brittle gypsum board, and it stands out particularly for its characteristics of high impact strength and high modulus of rupture.
Keywords: gypsum-cellulose composite, waste fibers, recycled pulp, mechanical properties
The productive chain of the civil construction industry has represented one of the activities of the society which has interfered most directly with the environment. It is a large consumer of re-sources (materials/energy), highly polluting (emission of CO
a generator of residues. Therefore, in the search of a sustainable construction, attentions turn to research on agglomerates of minor energetic consumption and to the adequate use of industrial and agro-industrial waste. When compared to cement and lime, the industrial process of plaster production issues less anhydrous carbon (CO
and reveals the lowest energy consumption, being thus regarded as green agglomerate. However, studies carried out in this country indicate that the waste indexes of this material reach around 45% of the total dough1.
The combination of inorganic binder material such as gypsum with waste fibers has been considered an interesting option for mate-rial recycling and has been used for structural overlays and ceilings in several parts of the world2. The main advantage of using natural fibers is their high energy-absorbing capacity resulting from their low modulus of elasticity. When fiber pullout predominates over fracture, fiber-matrix bonding is considered the main factor influencing the composites toughness3, ensuring the possibility of post-fracture work, which is an important characteristic in civil construction. The high availability of noncommercial fiber waste4, or low cost fibers, may constitute a good opportunity for a serious proposal of sustainable methods for producing low cost gypsum-fiber components for civil
construction. Compared to composites reinforced with virgin fibers, composites containing recycled fibers have presented good mechani-cal properties. Research by Savastano Jr. et al.5 showed that banana pulp, Eucalyptus grandis and sisal wastes presented satisfactory adhesion in fiber-cement composites, reaching a flexural strength of 15.5 to 16.5 MPa. The sensitivity of natural fiber to the alkaline environment produced by the hydration of standard Portland cement with a pH of around 13 has led researchers6,7 to suggest the use of gypsum, with its pH of 7 to 8, as an adequate binder for matrices reinforced with alkaline-sensitive vegetal fibers.
The aim of this research was to examine the influence of cel-lulose pulp on the mechanical properties of construction gypsum. Moreover, the stirring vacuum de-watering process was evaluated for the production of composites. Savastano Jr Warden and Coutts8 previously studied and developed this technique for the production of composite materials based on cement matrices. The hydration kinetics and morphology of hardened paste are important parameters in understanding the material.
The hydration kinetics of gypsum occurs by an exothermic proc-ess of energy released in the form of heat. The microstructure of the paste changes in response to parameters such as hydration conditions, mixing water temperature, gypsum properties, and the application of chemical additives9. When gypsum is mixed with water, the super-saturated solution composed of SO
42 and Ca2+ ions precipitates into a
needle-like crystalline network in a matter of minutes. Hardening be-
392 Carvalho et al. Materials Research
gins at the instant when the temperature gradient exceeds 0.1 C/min and ends when the temperature reaches its maximum10. The reactivity of the hydration can be quantified based on calorimetric curves, i.e., on the velocity of heat radiation.
For the morphological analysis, fractured gypsum surfaces, with and without addition of cellulose pulp were prepared and visualised through a scanning electron microscope (SEM). The kinetics of the hydration process was assessed using a pseudo-adiabatic calorim-eter.
The materials used in this work were natural gypsum (NG), recycled gypsum (RG), limestone, Kraft paper pulp from discarded cement bags (cel-cb), and water (Figure 1).
The natural gypsum (NG) used in this research is a commercial product from the region of Graja, Maranho state, Brazil, com-mercially available on the construction materials market, while the recycled gypsum (RG) originated from construction debris (dehy-drated at 85 C in a fan-assisted oven and milled for 20 minutes in ball-type mill). Table 1 lists the chemical composition and physical properties of the materials.
Calcium sulfates are the main components of gypsum. When treated with a diluted chloric acid solution they are expressed as sulfuric anhydride (SO
3) and calcium oxide (CaO), while impurities
such as quartz are expressed as insoluble residues (RI). Clay min-erals are quantifiable as aluminum (Al
3) and iron (Fe
contents. Table 1 indicates that the products used here were of high purity grade, i.e., SiO
3 < 1.5%.
With regard to the calcium oxide content (CaO = 38.65%), the product fell within the standard limits. The sulfuric anhydride did not
meet the Brazilian standard11, but lay within the limits established by the British12 and French13 standards, which admit minimum values of respectively. Cincotto et al.14 analyzed 15 different types of Brazil-ian gypsum and concluded that a minimum value of 50% for SO
sufficient to ensure gypsum quality.Limestone is a raw material commonly employed by cement and
fiber-cement manufacturers. The limestone used here came from the municipality of Cesarina, Gois state, Brazil, and was supplied by Eternit Ltda. Its probable chemical composition is given in Table 2.
The limestone used here an inert additive that facilitates drain-age of the paste during molding had a low fineness factor, with 67.5% of the particles sifting through a 100 mesh sieve, 18% through a 200 mesh sieve and 0.7% through a 325 mesh sieve. 17.3% of the particles were retained in the latter sieve and were added to the gypsum mass at a percentage of 10%.
The cellulose fibers of cement bag (cel-cb) were dispersed with water in a hydropulper, a giant industrial blender that separates parti-cles, blending them into a homogeneous pulp. This preparation took place in the following stages: at a concentration of 6 g of Kraft paper per liter of potable water, the material was processed for 30 minutes (this period was established during the pulping process, since it resulted in the best pulp dispersion quality). After this dispersion process, the excess was drained off through a sieve and a fine strainer (causing the pulp to reagglomerate). Lastly, the pulp, with a moisture content of about 75%, was again mixed for 5 minutes in a low speed laboratory electric mixer and stored in plastic bags in a refrigerator.
Table 1. Chemical and physical characteristics of the natural (NG) and recycled (RG) gypsum.
Properties Standards - limits Natural gypsum (NG)
Recycled gypsum (RG)NBR 13207 BS 1191/73 NFB 12300/63
Chemical analysis (%)
Water of crystallization 4.2 to 6.2 - - 7.91 10.65
CaO >38 23.3 - 38.65 35.94SO
3 >53 35 >45 52.08 49.61
3- - - 0.41 0.45
SiO2 + RI - - - 0.65 0.85
Calculated chemical percentage (%)
2O) - - - 92.22 91.12
(CaSO4) - - - - -
2O) 3.3 4.6
pH - - - - 7.96 8.12
Specific mass (g.cm3) > 700.00 2.50 2.56
Unit mass (kg.m